Synthesis, Characterization, and Catalytic Performance of Highly Dispersed Co-SBA-15
Chuan Wang, Sangyun Lim, Guoan Du, Codruta Zoican Loebicki, Nan Li, Salim Derrouiche,and Gary L. Haller*Department of Chemical Engineering, Yale UniVersity, P.O. Box 208286, New HaVen, Connecticut 06520-8286
ReceiVed: February 27, 2009; ReVised Manuscript ReceiVed: June 19, 2009
Highly dispersed cobalt on SBA-15 was successfully prepared by a post synthesis grafting of cobalt. Of thecobalt precursors tested, Co(II) acetylacetonate was found to be the best source for high dispersion of cobalt.The Co-SBA-15 catalysts were characterized with different techniques: N2 physisorption, XRD, TPR, TEM,and X-ray adsorption analysis. The mesoporous structure of SBA-15 was retained after cobalt grafting withup to 10 wt % Co loading. There were no large cobalt oxide particles formed, which indicates all the cobaltions are highly dispersed on the surface and the direct bonding to the silica surfaces results in a high reductiontemperature (1123 K) relative to Co oxides. X-ray absorption analysis demonstrates a local structure of Coions with all Co ions isolated and bonded with oxygen. XANES analysis requires that the local environmentfor Co ions be that of either a distorted tetrahedral or an octahedral structure and the fitting of EXAFS datafurther shows a Co-O bond coordination number of 3.58 ( 0.48, confirming that the Co is in a distortedtetrahedral environment. The catalytic activity of Co-SBA-15 catalyst was studied for the synthesis of carbonsingle walled nanotubes (SWNT). The high reduction stability of Co-SBA-15 is presumed to make a favorablecatalyst for this high temperature reaction. Raman spectroscopy and TEM photographs show that good qualitycarbon SWNT was synthesized by Co-SBA-15. Moreover, Co-SBA-15 has a higher yield of carbon SWNTcompared with Co-MCM-41 (C16 alkyl template) under the same reaction conditions.
Cobalt-incorporated (during synthesis) mesoporous catalystCo-MCM-41 was recently demonstrated to be a good catalystfor the synthesis of carbon single-walled nanotubes (SWNT).14
It is believed that the growth mechanism of carbon SWNT onCo-MCM-41 catalyst involves reduced cobalt metal particlesacting as the catalytic sites for both dissociation of CO andaggregation of carbon atoms to form the carbon SWNT.5 Themost important step is to control the particle size of the reducedcobalt because carbon SWNT can only grow from small cobaltparticles6 and the diameter of the SWNT is primarily controlledby the cobalt particle size.710 A narrow diameter distributionis desired, and this requires small and stable cobalt particles ofuniform size. In Co-MCM-41, cobalt ions (as Co2+) aresubstituted for silicon in the MCM-41 silica framework, whichresults in a high dispersion of cobalt ions. It has beendemonstrated by X-ray absorption analysis that essentially allcobalt ions are isolated in the MCM-41 silica matrix. Analysisof EXAFS data shows that cobalt ions are bonded directly withonly oxygen atoms (which in turn, are bonded to silicon cations)in a distorted tetrahedral surrounding and there is no measurableCo-Co bonding. The high dispersion of cobalt ions with highstability is correlated with a high reduction temperature. Themaximum reduction temperature of Co-MCM-41 (made fromC16 alkyl template) is about 1033 K. Such high reductionstability also makes Co-MCM-41 a preferred catalyst for thesynthesis of carbon SWNT by CO disproportionation, which isa high-temperature reaction (973-1023 K). In early work, theyield of carbon SWNT was only about 3 wt % using 3 wt %Co-MCM-41 (C16 alkyl template).11 A route to increase theyield of carbon SWNT is to increase cobalt loading. However,
there is a limit of cobalt loading in Co-MCM-41 because themesoporous structure starts to collapse when the cobalt loadingexceeds 4 wt %.12 This is partly due to the thin wall of theMCM-41 structure. Thus, we wish to find another support whichgives not only high dispersion and high reduction stability ofcobalt ions, but also has a high cobalt loading. That is, smallCo metal particles are desired for SWNT synthesis, and theseare difficult to stabilize against sintering at the high temperaturesrequired for CO disproportionation to SWNT. One mechanismof stabilization against sintering is anchoring Co metal particlesto Co cations in a silica matrix,13 so that anchoring potential isincreased when Co cations have a high reduction stability.
SBA-15 is a mesoporous material similar to MCM-41 buthas larger pores and thicker walls.14 The synthesis conditionsused to prepare SBA-15 are different from MCM-41. SBA-15materials are synthesized using a triblock polymer as a structure-directing agent and tetraethylorthosilicate as a silica source underacid conditions14,15 while MCM-41 materials are synthesizedunder extremely basic conditions by a sol-gel method. Thedifferent synthesis conditions make it difficult to synthesize Co-SBA-15 in the same way as Co-MCM-41. Co-MCM-41 wassynthesized by simply adding cobalt precursors during thesynthesis of siliceous MCM-41. However, this method does notwork for Co-SBA-15 because there is very limited solubilityof Co salts in the solution required to dissolve the polymer,e.g., pH < 2. Essentially all cobalt ions remain unreacted in theliquid phase after the synthesis. Increasing the pH of thesynthesis solution is not an option because the mesoporousstructure of SBA-15 cannot be maintained at pH values higherthan 2. An alternate method to introduce cobalt into SBA-15support is required.
One of the most commonly used methods for making metaloxide catalyst is impregnation. Cobalt contained SBA-15catalysts have been synthesized by the impregnation method
* To whom correspondence should be addressed: E-mail: email@example.com. Phone: 1-203-432-4378. Fax: 1-203-432-4387.
J. Phys. Chem. C 2009, 113, 1486314871 14863
10.1021/jp901823v CCC: $40.75 2009 American Chemical SocietyPublished on Web 07/23/2009
with different cobalt precursors.16,17 However, impregnated Co-SBA-15 showed low dispersion of cobalt ions and low reductionstability. The reduction temperature of impregnated cobalt Co-SBA-15 is around 723 K, which is the reduction temperatureof surface cobalt oxide. Such impregnated Co-SBA-15 is notuseful in the synthesis of carbon SWNT because all the cobaltions will be reduced and aggregated into large particles (tensof nanometers) at high reaction temperature.
Another approach for the creation of supported metal oxidecatalysts, recognized as molecular designed dispersion (MDD)or atomic layer deposition (ALD), which consists of theadsorption and subsequent thermolysis of supported metalacetylacetonate (Mn+(acac)n) complexes (or similar precursors)has been studied in the last two decades.1827 We call it a graftingmethod here because a metal precursor is grafted on the surfaceof the support and will be incorporated into the surface aftercalcination. Such a MDD or ALD method for the synthesis ofsupported metal oxide catalysts consists of two steps: (i)irreversible adsorption of the complex by hydrogen bonding orby a ligand exchange mechanism and (ii) decomposition of thegrafted complex in an oxygen-containing atmosphere at elevatedtemperatures. The process of this grafting method is visualizedin Figure 1. There are two possible pathways for the adsorptionof the complexes: (i) through hydrogen bonding between anacetylacetonate ligand and the surface hydroxyls or (ii) by ligandexchange in which a covalent metal-oxygen support bond isformed while an acetylacetonate ligand (Hacac) is lost. Van DerVoort has proved the first pathwayshydrogen bonding for theadsorption of VO(acac)2 on silica.21 He defined an R value asthe ratio of adsorbed acac ligands to the adsorbed vanadiumspecies. If the adsorption mechanism is hydrogen bonding,the R value should be 2. Otherwise, R is 1 for the ligandexchange pathway. Their experimental results showed thatR was 2, which proved the hydrogen bonding mechanism.Some other work also confirmed this mechanism for theadsorption of metal acetylacetonate.22,28
Recently, Iglesia and co-workers used a similar graftingmethod for the synthesis of highly dispersed tungsten oxidecatalyst on mesoporous silica.29 They used organic solvents andanhydrous conditions to control the deposition of tungsten oxidespecies onto the silica surface. In our work, Co-SBA-15 wassynthesized by a two-step method combining the synthesis ofsiliceous SBA-15 and then deposition of cobalt ions onto SBA-15 using the grafting method with different Co complexes. Thesynthesized Co-SBA-15 was characterized by different tech-niques to demonstrate the high dispersion of cobalt ions andhigh reduction stability, e.g., XRD, N2 physisorption, TEM, andTPR. X-ray absorption experiments were conducted to helpunderstand the local environment of cobalt ions in the synthe-sized Co-SBA-15 catalyst and the reduction to metal. Thecatalytic efficiency of Co-SBA-15 was tested with our desired
reaction, carbon SWNT synthesis. Raman spectra and TEMphotographs showed the production of good quality carbonSWNT. Also, because higher cobalt loading was attained, ahigher yield of carbon SWNT was achieved compared withthe original Co-MCM-41 catalyst under the same reactionconditions.14
2. Experimental Section
2.1. Preparation of Catalysts. The cobalt-grafted SBA-15catalysts were synthesized following a two-step method. First,mesoporous siliceous SBA-15 was synthesized according to aprocedure described by Stucky and co-workers using a triblockcopolymer (EO20PO70EO20, P123, Aldrich) as the structuredirecting agent and tetraethylorthosilicate (TEOS, Aldrich, 98%)as the silica source under acidic conditions.14,15 Four grams ofthe EO20PO70EO20 was dissolved in 30 g of H2O and 120 g of2 M HCl. The mixture was continually stirred until thecopolym